FSC 9310 JCP A50
MACHINE-FINISH BOOK END
Printing Paper February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For end leaves of bound books, some of which may be printed by the offset process. Printed matter may include line illustrations
and halftones up to 150-lines screen.
Unless the option below is specified, the following ‘basic’ specification applies.
Stock: Groundwood pulp, not to exceed 10 pct. General appearance: Paper shall conform to the standard sam-
Note: 1 Not less than 30 postconsumer fiber. Any percent over ple(s) adopted by the Government.
30 percentage points, is encouraged, provided that the require- Color: The paper in the order (or publication) shall be uniform
ments of this Standard are met. with a target brightness of 72 pct ±2 pct or as specified. The
color variation shall not exceed DE(CIELAB)=1.0.
Grammage (g/m2) ................................................................ 120
Basis weight: 25 by 38 inches, 500 sheets (pounds) ....... 80 Finish and formation: Shall be uniform.
A tolerance of ±5 pct shall be allowed. Cleanliness: The dirt count for each side of the paper shall not
exceed 250 specks per square meter. No sample sheet (600 to
Folding endurance: Average, each direction, not less 650 cm2 in size) shall contain more than one defect with an
than— equivalent area of 0.25 mm2 or greater.
M.I.T. (double fold) ............................................................ 30
Schopper (double fold) ....................................................... 50 Sampling and testing: Shall be conducted in accordance with
standards in Part 2, Government Paper Specification Standards.
Option A: Alkaline paper. This option is for products requiring above average permanence.
The following requirements replace the same in the ‘basic’ specification and are added to the specification.
Stock: 100 pct bleached chemical woodpulp. Acidity: pH value by cold extraction shall be not less than 7.0.
The paper shall contain not less than 2 pct calcium carbonate.
Note: Postconsumer fiber, in any percentage, is encouraged, Any deviation in this requirement shall be sufficient cause for
provided that the requirements of this Standard are met. rejection of the paper.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Sizing: Paper shall be surface- and internal-sized suitable for sat- Size and trim: Sheets: Paper shall be furnished in the size(s) or-
isfactory printing on both sides of the paper on high-speed offset dered and shall be flat, trimmed square on four sides with clean
presses equipped with continuous flow or brush dampening sys- smooth edges, and evenly jogged. A tolerance of ±2 mm (1⁄16
tems. inch) shall be allowed except for sheets 216 by 356 mm (81⁄2 by
Color: Shall match the Government’s standard sample for color. 14 inches) or less; then a tolerance of ±1 mm (1⁄32 inch) shall be
A deviation of DE(CIELAB)±3.0 from the color standard is al- allowed. Successive sheets within any package shall not differ
lowed. from each other by more than 0.5 mm (1⁄64 inch). Paper with the
For information only, the CIELAB values (Ill D65, 10° ob- long dimension 813 mm (32 inches) or less shall be considered
server) of the white color standard are square if the variation does not exceed 1 mm (1⁄32 inch); over
L*=93.0 813 mm (32 inches), 2 mm (1⁄16 inch).
a*=¥0.5 Grain: Direction of the grain on flat paper shall be as ordered.
Curl: Paper shall lie flat with either no tendency to curl or with Pressroom conditions: The bulk of this paper will be used in
a curl which can be overcome under reasonable working condi- air-conditioned pressrooms maintained at 24 °C ±2 °C and 45 pct
tions. ±8 pct relative humidity.
1 This requirement may be waived by the ordering agency when purchasing less than a mill run quantity and so stated in the procure-